AASHTO Designation: T 307-99 (2012) Standard Method of Test for Determining the Resilient Modulus of Soils and Aggregate MaterialsDescripción completa
Descrição: AASHTO Designation: T 307-99 (2012) Standard Method of Test for Determining the Resilient Modulus of Soils and Aggregate Materials
Peugeot 307 EmulatorDescripción completa
A 29 - A 29M - 03 _QTI5LTAZFull description
Standard Specification for Zinc-Coated (Galvanized) Steel Bars for Concrete Reinforcement
ASTM A 123AFull description
Designation: A307 − 12
Standard Speciﬁcation for
Carbon Steel Bolts, Studs, and Threaded Rod 60 000 PSI Tensile Strength1 This standard is issued under the ﬁxed designation A307; the number immediately following the designation indicates the year of original origin al adoption or, in the case of revis revision, ion, the year of last revision. revision. A number in paren parenthese thesess indicates the year of last reappr reapproval. oval. A superscript epsilon (´) indicates an editorial change since the last revision or reapproval. This standard has been approved for use by agencies of the Department of Defense.
1. Sco Scope* pe* 1.1 This speciﬁcatio speciﬁcation n2 covers the chemical and mechanical requirements of two grades of carbon steel bolts and studs in sizes 1 ⁄ 4 in. through through 4 in. The fas fastene teners rs are des design ignated ated by “Grade” denoting tensile strength and intended use, as follows: Grade Grade A
Description Bolts, studs, and threaded rod having a minimum tensile strength of 60 ksi and intended for general applications, Bolts, studs, and threaded rodA having a tensile strength of 60 to 100 ksi and intended for ﬂanged joints in piping systems with cast iron ﬂanges, and Replaced by Speciﬁcation F1554 Gr.36 F1554 Gr.36
Threaded rod is not usually produced to Grade B, but can be when speciﬁed by the purchaser.
1.2 1. 2 Th This is sp spec eciﬁc iﬁcati ation on do does es no nott co cove verr re requ quir irem emen ents ts fo forr machine screws machine screws,, thread cutting/forming cutting/forming screws, mechan mechanical ical expansion anchors or similar externally threaded fasteners. 1.3 Suitab Suitable le nuts are covered in Speciﬁcation Speciﬁcation A563 A563.. Unless otherwise speciﬁed, the grade and style of nut for each grade of fastener, of all surface ﬁnishes, shall be as follows: Fastener Grade and Size A 1 ⁄ 4 to 11 ⁄ 2 in. A over 11 ⁄ 2 to 4 in. B, 1 ⁄ 4 to 4 in.
Nut Grade and StyleA A, h e x A , h e av y h ex A , h e av y h ex
Nuts of other grades and styles having speciﬁed proof load stresses (Speciﬁcation A563, A563, Table 3) greater than the speciﬁed grade and style of nut are also suitable.
1.4 The values stated in inch-poun inch-pound d units are to be regar regarded ded as the standard.
1.5 Suppl Supplementar ementary y Requirement Requirement S1 of an optional nature is provided, prov ided, which describ describes es additi additional onal restrictions restrictions to be applie applied d when bolts are to be welded. It shall apply only when speciﬁed in the inquiry, order, and contract. 1.6 Term ermss use used d in thi thiss spe speciﬁc ciﬁcatio ation n are deﬁ deﬁned ned in Term ermiinology F1789 nology F1789 unless otherwise deﬁned herein. 2. Referenc Referenced ed Documents 2.1 ASTM Standards: 3 A563 Speciﬁcation A563 Speciﬁcation for Carbon and Alloy Steel Nuts A706/A706M Speciﬁcation A706/A706M Speciﬁcation for Low-Alloy Steel Deformed and Plain Bars for Concrete Reinforcement A751 Test A751 Test Methods, Practices, and Terminology for Chemical Analysis of Steel Products B695 Speciﬁcation B695 Speciﬁcation for Coatings of Zinc Mechanically Deposited on Iron and Steel F606 Test F606 Test Methods for Determining the Mechanical Properties of Ext Extern ernally ally and Int Intern ernally ally Thr Thread eaded ed Fas Fastene teners, rs, Washers, Direct Tension Indicators, and Rivets F1470 Pra Practic cticee for Fas Fasten tener er Sam Sampli pling ng for Spe Speciﬁe ciﬁed d Mechanicall Prope chanica Properties rties and Perfo Performance rmance Inspection F1554 Spe Speciﬁc ciﬁcatio ation n for Anchor Anchor Bol Bolts, ts, Ste Steel, el, 36, 55, and 105-ksi Yield Strength F1789 Terminology for F16 Mechanical Fasteners F1789 F2329 Spe Speciﬁc ciﬁcatio ation n for Zin Zincc Coat Coating ing,, Hot Hot-Di -Dip, p, Req Requir uireements for Application to Carbon and Alloy Steel Bolts, Screws, Washers, Nuts, and Special Threaded Fasteners 2.2 ASME Standards: B 1.1 Uniﬁed Screw Threads4 B 18.2.1 Square 18.2.1 Square and Hex Bolts and Screws 4 B 18.24 Part 18.24 Part Identifying Number (PIN) Code System 5 B18.31.3 Threaded B18.31.3 Threaded Rods (Inch Series)4
This speciﬁcation speciﬁcation is under the jurisd jurisdictio iction n of ASTM Commi Committee ttee F16 on Fasteners Faste ners and is the direct respo responsibil nsibility ity of Subco Subcommitte mmitteee F16.02 on Steel Bolts, Nuts, Rivets and Washers. Current Curre nt editio edition n appro approved ved Dec. 1, 2012. Published Published Janua January ry 2013. Originally Originally approved approv ed in 1947. Last previous edition edition approv approved ed in 2010 as A307 –10. DOI: 10.1520/A0307-12. 2 For ASME Boiler and Pressure Vessel Code applications see related Speciﬁcation SA-307 in Section II of that Code.
For referenced ASTM standards, visit the ASTM website, www.astm.org, or contact ASTM Customer Service at [email protected] For Annual Book of ASTM Standards volume information, refer to the standard’s Document Summary page on the ASTM website. 4 Available from American National Standards Institute (ANSI), 25 W. 43rd St., 4th Floor, New York, NY 10036, http://www.ansi.org. 5 Availab vailable le from American Soci Society ety of Mecha Mechanical nical Engin Engineers eers (ASM (ASME), E), ASME International Headquarters, Three Park Ave., New York, NY 10016-5990, http:// www.asme.org.
Copyright by ASTM Int'l (all rights reserved); reserved); Thu Feb 7 07:18:06 EST 2013 1 Downloaded/printed by MC MASTER UNIVERSITY pursuant to License Agreement. No further reproductions authorized.
A307 − 12 3. Ordering Information 3.1 Orders for externally threaded fasteners (including nuts and accessories) under this speciﬁcation shall include the following: 3.1.1 ASTM designation and year of issue, 3.1.2 Name of product, bolts or studs; and bolt head style, that is, hex or heavy hex, or threaded rod, 3.1.3 Grade, that is, A, or B. If no grade is speciﬁed, Grade A is furnished. 3.1.4 Quantities (number of pieces by size including nuts), 3.1.5 Fastener size and length, 3.1.6 Washers— Quantity and size (separate from bolts), 3.1.7 Zinc Coating— S pecify the zinc-coating process required, for example, hot-dip, mechanically deposited, or no preference (see 4.5). 3.1.8 Other Finishes— Specify other protective ﬁnish, if required. 3.1.9 Specify if inspection at point of manufacture is required, 3.1.10 Specify if certiﬁed test report is required (see 8.2), and 3.1.11 Specify additional testing (8.3) or special requirements. 3.1.12 For establishment of a part identifying system, see ASME B18.24. 4. Materials and Manufacture 4.1 Steel for bolts, studs, and threaded rod shall be made by the open-hearth, basic-oxygen, or electric-furnace process. 4.2 Bolts shall be produced by hot or cold forging of the heads or machining from bar stock. 4.3 Heat Treatment: 4.3.1 Cold headed fasteners with head conﬁgurations other than hex having a minimum head height less than or equal to .5 D (D is nominal diameter) shall be stress relief annealed at a minimum temperature of 875°F. 4.3.2 Stress relieving of hex head fasteners and those with minimum head heights greater than .5 D shall be at the manufacturer’s option. 4.4 Bolt and stud threads shall be rolled or cut. 4.5 Zinc Coatings, Hot-Dip and Mechanically Deposited: 4.5.1 When zinc-coated fasteners are required, the purchaser shall specify the zinc-coating process, for example hot dip, mechanically deposited, or no preference. 4.5.2 When hot-dip is speciﬁed, the fasteners shall be zinc-coated by the hot-dip process in accordance with the requirements of Speciﬁcation F2329. 4.5.3 When mechanically deposited is speciﬁed, the fasteners shall be zinc-coated by the mechanical-deposition process in accordance with the requirements of Class 55 of Speciﬁcation B695. 4.5.4 When no preference is speciﬁed, the supplier may furnish either a hot-dip zinc coating in accordance with Speciﬁcation F2329, or a mechanically deposited zinc coating in accordance with Speciﬁcation B695, Class 55. Threaded components (bolts and nuts) shall be coated by the same
zinc-coating process and the supplier’s option is limited to one process per item with no mixed processes in a lot. 5. Chemical Composition 5.1 Grade A and B bolts, studs, and threaded rod shall have a heat analysis conforming to the requirements speciﬁed in Table 1 based on the steel producer’s heat analysis. 5.2 The purchaser shall have the option of conducting product analyses on ﬁnished bolts in each lot, which shall conform to the product analysis speciﬁed in Table 1. 5.3 In case of conﬂict or for referee purposes, the product analysis shall take precedence. 5.4 Bolts and studs are customarily furnished from stock, in which case individual heats of steel cannot be identiﬁed. 5.5 Application of heats of steel to which bismuth, selenium, tellurium, or lead has been intentionally added shall not be permitted for Grade B bolts and studs. 5.6 Chemical analyses shall be performed in accordance with Test Methods, Practices, and Terminology A751. 6. Mechanical Properties 6.1 Grades A and B bolts, studs, and threaded rod shall conform to the hardness speciﬁed in Table 2. 6.2 Grade A and B bolts, studs, and threaded rod 1½ in. in diameter or less, other than those excepted in 6.4, shall be tested full size and shall conform to the requirements for tensile strength speciﬁed in Table 3. Threaded rod is permitted to be cut to a length suitable for tensile testing and shall be treated using the same method speciﬁed for studs. 6.3 Grade A and B bolts, studs, and threaded rod larger than 1 ⁄ 2 in. in diameter, other than those excepted in 6.4, shall preferably be tested full size and when equipment of sufficient capacity is available and shall conform to the requirements for tensile strength speciﬁed in Table 3. When equipment of sufficient capacity for full-size testing is not available, or when the length of the bolt or stud makes full-size testing impractical, machined specimens shall be tested and shall conform to the requirements speciﬁed in Table 4. 1
6.4 Grades A and B bolts and studs less than three diameters in length or bolts with drilled or undersize heads are not subject to tensile tests. 6.5 In the event that bolts, studs, and threaded rod are tested by both full size and by machine test specimen methods, the full-size test shall govern if a controversy between the two methods exists. TABLE 1 Chemical Requirements for Grades A and B Bolts, Studs, and Threaded Rod Carbon, max Manganese, max Phosphorus, max Sulfur, max Grade A Grade B A
Heat Analysis 0.29 1.20 0.04
Product Analysis 0.33 1.25 0.041
Resulfurized steel is not subject to rejection based on product analysis for sulfur.
Copyright by ASTM Int'l (all rights reserved); Thu Feb 7 07:18:06 EST 2013 2 Downloaded/printed by MC MASTER UNIVERSITY pursuant to License Agreement. No further reproductions authorized.
A307 − 12 TABLE 2 Hardness Requirements for Bolts, Studs, and Threaded Rod Grade
Less than 3 × diaB 3 × dia and longer Less than 3 × diaB 3 × dia and longer
121 ... 121 ...
241 241 212 212
69 ... 69 ...
100 100 95 95
As measured anywhere on the surface or through the cross section. Also bolts with drilled or undersize heads. These sizes and bolts with modiﬁed heads shall meet the minimum and maximum hardness as hardness is the only requirement. B
TABLE 3 Tensile Requirements for Full-Size Bolts, Studs, and Threaded Rod Threads per inch
Stress Area,A in.2
Tensile Strength, lbfB Grade A, min C
Grade B minD
⁄ 4 ⁄ 16 3 ⁄ 8 7 ⁄ 16
20 18 16 14
0.0318 0.0524 0.0775 0.1063
1 3 4 6
900 100 650 350
1 3 4 6
900 100 650 350
3 5 7 10
180 240 750 630
⁄ 2 ⁄ 16 5 ⁄ 8 3 ⁄ 4 7 ⁄ 8
13 12 11 10 9
0.1419 0.182 0.226 0.334 0.462
8 11 13 20 27
500 000 550 050 700
8 11 13 20 27
500 000 550 050 700
14 18 22 33 46
190 200 600 400 200
1 11 ⁄ 8 11 ⁄ 4 13 ⁄ 8
8 7 7 6
0.606 0.763 0.969 1.155
36 45 58 69
350 800 150 300
36 45 58 69
350 800 150 300
60 76 96 115
600 300 900 500
11 ⁄ 2 13 ⁄ 4 2 21 ⁄ 4
6 5 4½ 4½
1.405 1.90 2.50 3.25
84 114 150 195
300 000 000 000
84 114 150 195
300 000 000 000
140 190 250 325
500 000 000 000
21 ⁄ 2 23 ⁄ 4 3 31 ⁄ 4
4 4 4 4
4.00 4.93 5.97 7.10
240 295 358 426
000 800 200 000
240 295 358 426
000 800 200 000
400 493 597 710
000 000 000 000
31 ⁄ 2 33 ⁄ 4 4
4 4 4
8.33 9.66 11.08
499 800 579 600 664 800
499 800 579 600 664 800
833 000 966 000 1 108 000
Area calculated from the equation: As = 0.7854 [D − (0.9743/ n) ] where: As = D = n =
Tensile strength, ksi Yield point, min ksi Elongation in 2 in., min, %
Bolt Size, in.
60 min ... 18
60–100 ... 18
TABLE 4 Tensile Requirements for Machined Specimens
stress area, nominal diameter of bolt, and threads per inch.
7. Dimensions 7.1 Unless otherwise speciﬁed, threads on bolts and studs shall be the Coarse Thread Series as speciﬁed in the latest issue of ASME B1.1, and shall have a Class 2A tolerance. Unless otherwise speciﬁed, threads on threaded rod shall be per the requirements of the latest issue of ASME B18.31.3. 7.2 Unless otherwise speciﬁed, Grade A bolts shall be hex bolts with dimensions as given in the latest issue of ASME B18.2.1. Unless otherwise speciﬁed, Grade B bolts shall be heavy hex bolts with dimensions as given in the latest issue of ASME B18.2.1. Unless otherwise speciﬁed, threads on threaded rod shall be per the requirements of the latest issue of ASME B18.31.3. 7.3 Unless otherwise speciﬁed, bolts, studs, and threaded rod to be used with nuts or tapped holes which have been tapped oversize, in accordance with Speciﬁcation A563, shall have threads as speciﬁed in 7.1 before hot-dip or mechanically deposited zinc coating. After zinc coating the maximum limit of pitch and major diameter shall not exceed the Class 2A maximum limit by more than the following amounts: Diameter, in. ⁄ 4 ⁄ 16, 3 ⁄ 8 7 ⁄ 16, 1 ⁄ 2 9 ⁄ 16 to 3 ⁄ 4, incl 7 ⁄ 8 1.0 to 11 ⁄ 4, incl 13 ⁄ 8, 11 ⁄ 2 13 ⁄ 4 to 4.0, incl 1
These values are the same as the overtapping required for zinc-coated nuts in Speciﬁcation A563.
7.4 The gaging limit for bolts and studs, and threaded rod shall be veriﬁed during manufacture or use by assembly of a nut tapped as nearly as practical to the amount oversize shown above. In case of dispute, a calibrated thread ring gage of that same size (Class X tolerance, gage tolerance plus) shall be used. Assembly of the gage, or the nut described above, must be possible with hand effort following application of light machine oil to prevent galling and damage to the gage. These inspections, when performed to resolve disputes, shall be performed at the frequency and quality described in Table 5.
1 lbf = 4.448 N. Based on 60 ksi (414 MPa). D Based on 60–100 ksi (414–690 MPa). C
6.6 For bolts, studs, and threaded rod on which both hardness and tension tests are performed, acceptance based on tensile requirements shall take precedence in the event that there is controversy over low readings of hardness tests.
8. Number of Tests and Retests 8.1 The requirements of this speciﬁcation shall be met in continuous mass production for stock, and the manufacturer shall make sample inspections to ensure that the product conforms to the speciﬁed requirements. Additional tests of individual shipments of material are not ordinarily contemplated. Individual heats of steel are not identiﬁed in the ﬁnished product.
Copyright by ASTM Int'l (all rights reserved); Thu Feb 7 07:18:06 EST 2013 3 Downloaded/printed by MC MASTER UNIVERSITY pursuant to License Agreement. No further reproductions authorized.
A307 − 12 TABLE 5 Sample Sizes and Acceptance Numbers for Inspection of Hot-Dip or Mechanically Deposited Zinc-Coated Threads Lot Size
be made before shipment, and shall be conducted as not to interfere unnecessarily with the operation of the works.
11. Responsibility 2 to 90 91 to 150 151 to 280 281 to 500 501 to 1 200 1 201 to 3 200 3 201 to 10 000 10 001 and over A
13 20 32 50 80 125 200 315
1 2 3 5 7 10 14 21
Inspect all bolts in the lot if the lot size is less than the sample size.
11.1 The party responsible for the fastener shall be the organization that supplies the fastener to the purchaser. 12. Rejection and Rehearing 12.1 Disposition of nonconforming lots shall be in accordance with Guide F1470, speciﬁcally sections on disposition of nonconforming lots, suppliers option, and purchasers option. 13. Product Marking
8.2 When speciﬁed in the order, the manufacturer shall furnish a test report certiﬁed to be the last completed set of mechanical tests for each stock size in each shipment. 8.3 When additional tests are speciﬁed on the purchase order, a lot, for purposes of selecting test samples, shall consist of all material offered for inspection at one time that has the following common characteristics: 8.3.1 One type of item, 8.3.2 One nominal size, and 8.3.3 One nominal length of bolts and studs. 8.4 From each lot, the number of tests for each requirement shall be as follows: Number of Pieces in Lot 800 and under 801 to 8 000 8 001 to 22 000 Over 22 000
Number of Samples 1 2 3 5
8.5 If any machined test specimen shows defective machining it shall be discarded and another specimen substituted. 8.6 Should any sample fail to meet the requirements of a speciﬁed test, double the number of samples from the same lot shall be tested, in which case all of the additional samples shall meet the speciﬁcation. 9. Test Methods 9.1 Grades A and B bolts and studs shall be tested in accordance with Test Methods F606. 9.2 Standard square and hex head bolts only shall be tested by the wedge tension method except as noted in 6.4. Fracture shall be in the body or threads of the bolt without any fracture at the junction of the head and body. Other headed bolts shall be tested by the axial tension method. 10. Inspection 10.1 If the inspection described in 10.2 is required by the purchaser it shall be speciﬁed in the inquiry, order, or contract. 10.2 The inspector representing the purchaser shall have free entry to all parts of the manufacturer’s works that concern the manufacture of the material ordered. The manufacturer shall afford the inspector all reasonable facilities to satisfy him that the material is being furnished in accordance with this speciﬁcation. All tests and inspections required by the speciﬁcation that are requested by the purchaser’s representative shall
13.1 Grades A and B Bolts and Studs: 13.1.1 Bolt heads and one end of studs shall be marked with a unique identiﬁer by the manufacturer to identify the manufacturer or private label distributor, as appropriate. Additional marking required by the manufacturer shall be at the option of the manufacturer. 13.1.2 In addition to the requirements of 13.1, all bolt heads, one end of studs ⅜ in. and larger, and whenever feasible studs less than ⅜ in. shall be marked with a grade marking as follows: Grade A B
Marking 307A 307B
13.1.3 All markings shall be located on the top of the bolt head or stud end and shall be raised or depressed at the option of the manufacturer. 13.2 Grades A and B Threaded Rod: 13.2.1 Refer to ASME B18.31.3 for marking of Grade A and B threaded rod. 13.2.2 If markings are required, they shall be located on the ends of the threaded rod and shall be raised or depressed at the option of the manufacturer. 14. Packaging and Package Marking 14.1 Packaging: 14.1.1 Unless otherwise speciﬁed, packaging shall be in accordance the manufacturer’s practice to prevent damage before and during shipment. 14.1.2 When special packaging requirements are required, they shall be deﬁned at the time of the inquiry and order. 14.2 Package Marking: 14.2.1 Each shipping unit shall include or be plainly marked with the following information: 126.96.36.199 ASTM designation and grade, 188.8.131.52 Size, 184.108.40.206 Name and brand or trademark of the manufacturer, 220.127.116.11 Number of pieces, 18.104.22.168 Purchase order number (when speciﬁed in the order), 22.214.171.124 Country of origin. 15. Keywords 15.1 all thread rod; bolts; carbon steel; steel; studs; threaded rod
Copyright by ASTM Int'l (all rights reserved); Thu Feb 7 07:18:06 EST 2013 4 Downloaded/printed by MC MASTER UNIVERSITY pursuant to License Agreement. No further reproductions authorized.
A307 − 12 SUPPLEMENTARY REQUIREMENTS The following supplementary requirement shall apply only when speciﬁed in the purchase order or contract:
S1. Bolts Suitable for Welding S1.1 The material described in this section is intended for welding. This supplemental section, by additional chemical composition restrictions and by a carbon equivalent formula, provides assurance of weldability by chemical composition control. S1.2 Welding technique is of fundamental importance when bolts produced to this supplementary section are welded. It is presupposed that suitable welding procedures for the steel being welded and the intended service will be selected. S1.3 All of the requirements of this supplemental section apply in addition to all of the chemical, mechanical, and other requirements of the base speciﬁcation, Speciﬁcation A307 for Grade B. S1.4 Because of the embrittling effects of welding temperatures on cold-forged steel, this supplemental section is limited to hot-forged bolts, or, if not forged, then to bolts produced from hot-rolled bars without forging or threaded bars, bars studs, or stud bolts produced from hot-rolled bars without forging. Cold-forged bolts, or cold-drawn threaded bars, if they are given a thermal treatment by heating to a temperature of not less than 1500°F (815°C) and air-cooled are also suitable. S1.5 Chemical Requirements: S1.5.1 Heat Chemical Analysis—Material conforming to the following additional analysis limitations shall be used to manufacture the product described in this supplementary requirement. Carbon Manganese Phosphorus Sulfur Silicon
0.30 %, 1.00 %, 0.04 %, 0.05 %, 0.50 %,
max max max max max
S1.5.2 Carbon Equivalent (Source—Speciﬁcation A706/ A706M )—In addition to the heat chemical analysis requirements in S1.5.1, the heat analysis shall be such as to provide a carbon equivalent (CE) not exceeding 0.55 when calculated as follows: CE 5 % C 1
% Mn 6
% Cu 40
% Ni 20
% Cr 10
% Mo 50
% V 10
S1.6 Analysis Reports—If requested on the order or contract, the chemical composition of each heat of steel used and the calculated carbon equivalent for each heat shall be reported to the purchaser. S1.7 Product (Check) Veriﬁcation Analysis —Chemical analyses when made by the purchaser or a representative on bolts from each heat of steel, shall not exceed the values speciﬁed in S1.5.2 by more than the following amounts: Carbon Manganese Phosphorus Sulfur Silicon
% +0.03 +0.06 +0.008 +0.008 +0.05
S2. Permanent Manufacturer’s Identiﬁcation S2.1 Replaced by Speciﬁcation F1554. S3. Permanent Grade Identiﬁcation S3.1 Replaced by Speciﬁcation F1554.
SUMMARY OF CHANGES Committee F16 has identiﬁed the location of selected changes to this standard since the last issue (A307–10) that may impact the use of this standard. (1) Revised title to include threaded rod. (2) Added reference to threaded rod to sections, 1.1, 3.1.2, 4.1, 5.1, 6.1, 6.2, 6.3, 6.5, 6.6, 7.1, 7.2, 7.3, 7.4, and in Table 1, Table 2, and Table 3. (3) Removed section 9.3 as it is speciﬁed in Test Methods F606.
(4) Removed reference to Practice D3951 in section 2.1. (5) Added ASME B18.31.3 in 2.2. (6) Added 13.2. (7) Revised 14.1.1 and 126.96.36.199. (8) Added additional key words to Section 15.
Copyright by ASTM Int'l (all rights reserved); Thu Feb 7 07:18:06 EST 2013 5 Downloaded/printed by MC MASTER UNIVERSITY pursuant to License Agreement. No further reproductions authorized.
A307 − 12 ASTM International takes no position respecting the validity of any patent rights asserted in connection with any item mentioned in this standard. Users of this standard are expressly advised that determination of the validity of any such patent rights, and the risk of infringement of such rights, are entirely their own responsibility. This standard is subject to revision at any time by the responsible technical committee and must be reviewed every ﬁve years and if not revised, either reapproved or withdrawn. Your comments are invited either for revision of this standard or for additional standards and should be addressed to ASTM International Headquarters. Your comments will receive careful consideration at a meeting of the responsible technical committee, which you may attend. If you feel that your comments have not received a fair hearing you should make your views known to the ASTM Committee on Standards, at the address shown below. This standard is copyrighted by ASTM International, 100 Barr Harbor Drive, PO Box C700, West Conshohocken, PA 19428-2959, United States. Individual reprints (single or multiple copies) of this standard may be obtained by contacting ASTM at the above address or at 610-832-9585 (phone), 610-832-9555 (fax), or [email protected] (e-mail); or through the ASTM website (www.astm.org). Permission rights to photocopy the standard may also be secured from the ASTM website (www.astm.org/ COPYRIGHT/).
Copyright by ASTM Int'l (all rights reserved); Thu Feb 7 07:18:06 EST 2013 6 Downloaded/printed by MC MASTER UNIVERSITY pursuant to License Agreement. No further reproductions authorized.